The present work is a follow-up of the investigation on the decomposition reaction of kaolinite as a function of the defectivity of the starting material and the temperature of reaction. In the present work we study the high temperature reaction of mullite synthesis from kaolinite, from the starting point of the results obtained in the first part.
Time resolved energy-dispersive powder diffraction patterns have been measured using synchrotron radiation in isothermal conditions. The apparent activation energy for mullite nucleation and growth is found to be related to the defective structure of the starting kaolinite, which thus must have an influence on the chemical homogeneity of the amorphous intermediate phase.
The analysis of the kinetic data indicate that the initial reaction mechanism is controlled by mullite nucleation, while as the reaction proceeds it shifts towards a grain growth-limited process which is intermediate between phase boundary and diffusion controlled. The order of the reaction obtained from standard analysis of the isothermal kinetic data is lower in the case of the ordered kaolinite KGa-1, in agreement with a rate limiting process more strongly limited by diffusion.
For each sample there is a small but significant decrease in the order of the reaction at higher temperature: we interpret the change as related to the variation of the diffusion process in the amorphous phase due to the growing grains of mullite and cristobalite.
The values of the activation energies and induction times are comparable neither to a model of mullite formation from a monophasic gel, nor mullite formation from a diphasic gel, being intermediate between the two. We can infer that the amorphous precursors from natural kaolinites can be considered pseudo-monophasic gel-like phases, approaching the monophasic gel-like behaviour as the defectivity of the initial kaolinite increases.
This is a preview of subscription content, log in to check access.
Buy single article
Instant access to the full article PDF.
Price includes VAT for USA
Aksay IA, Pask JA (1975) Stable and metastable equilibria in the system SiO2-Al2O3. J Am Ceram Soc 58:507–512
Artioli G, Bellotto M, Gualtieri A, Pavese A (1995) Nature of structural disorder in natural kaolinites: a new model based on computer simulations of powder diffraction data and electrostatic energy calculations. Clays Clay Minerals, in press
Bamford CH, Tipper CFH (1980) Comprehensive chemical kinetics. Elsevier, New York 22:41-113
Bellotto M (1994) High temperature phase transitions in kaolinite: the influence of disorder and of kinetics on the reaction path. Mat Sci Forum Pt. 1 166:3–20
Bellotto M, Gualtieri A, Artioli G, Clark SM (1995) Kinetic study of the kaolinite-mullite reaction sequence. Part I: Kaolinite dehydroxylation. Phys Chem Minerals 22:207–214
Brindley GW, Nakahira M (1957) Kinetics of dehydroxylation of kaolinite and halloysite. J Am Ceram Soc 40:346–350
Brindley GW, Sharp JH, Patterson JH, Narahari BN (1967) Kinetics and mechanism of dehydroxylation processes. I. Temperature and vapor pressure dependence of dehydroxylation of kaolinite. Am Mineral 52:201–211
Clark SM (1989) Energy-dispersive powder diffraction at the SRS. Nucl Inst Meth Phys Res A276:381–387
Criado JM, Ortega A, Real C, Torres de Torres E (1984) Reexamination of the kinetics of the thermal dehydroxylation of kaolinite. Clay Minerals 19:653–661
Davis RF, Pask JA (1972) Diffusion reaction studies in the system Al2O3 -SiO2. J Am Ceram Soc 55:525–531
Donnay G, Wyart J, Sabatier G (1959) Structural mechanisms of thermal and compositional transformations in silicates. Z Kristallogr 112:161–168
Fripiat JJ, Toussaint F (1963) Dehydroxylation of kaolinite. II. Conductometric measurements and infrared spectroscopy. J Phys Chem 67:30–36
Goldsmith JR (1987) Al/Si interdiffusion in albite: effect of pressure and the role of hydrogen. Contrib Mineral Petrol 95:311–321
Goldsmith JR (1988) Enhanced Al/Si diffusion in KAlSi3O8 at high pressures: the effect of hydrogen. J Geology 96:109–124
Goldsmith JR, Jenkins DM (1985) The high-low albite relations revealed by reversal of degree of order at high pressures. Am Mineral 70:911–923
Hancock JD, Sharp JH (1972) Method of comparing solid-state kinetic data and its application to the decomposition of kaolinite, brucite, and BaCO3. J Am Ceram Soc 55:74–77
Johnson HB, Kessler F (1969) Kaolinite dehydroxylation kinetics. J Am Ceram Soc 52:199–204
Kriven WM, Pask JA (1983) Solid solution range and microstructures of melt-grown mullite. J Am Ceram Soc 66:649–654
Leonard AJ (1977) Structural analysis of the transition phases in the kaolinite-mullite thermal sequence. J Am Ceram Soc 60:37–43
Li DX, Thomson WJ (1990) Mullite formation kinetics of a singlephase gel. J Am Ceram Soc 73:964–969
Li DX, Thomson WJ (1991) Mullite formation from nonstoichiometric diphasic precursors. J Am Ceram Soc 74:2382–2387
MacKenzie KJD, Brown IWM, Meinhold RH, Bowden ME (1985) Outstanding problems in the kaolinite-mullite reaction sequence investigated by 29Si and 27Al solid-state nuclear magnetic resonance: I, metakaolinite. J Am Ceram Soc 68:293–297
Mazdiyasni KS, Brown LM (1972) Synthesis and mechanical properties of stoichiometric aluminum silicate (Mullite). J Am Ceram Soc 55:548–552
McIlvried HG, Massoth FE (1973) Effect of particle size distribution on gas-solid reaction kinetics for spherical particles. Ind Eng Chem Fundam 12:225–229
Murray P, White J (1949) Kinetics of thermal dehydration of clays. Trans Brit Ceram Soc 48:187–206
Murray P, White J (1955a) Kinetics of thermal dehydration characteristics of the clay minerals: I. Trans Brit Ceram Soc 54:137–150
Murray P, White J (1955 b) Kinetics of thermal dehydration characteristics of the clay minerals: II. Trans Brit Ceram Soc 54:151–187
Murray P, White J (1955c) Kinetics of thermal dehydration characteristics of the clay minerals: III. Trans Brit Ceram Soc 54:204–238
Okada K, Otsuka N (1986) Characterization of the spinel phase from SiO2-Al2O3 xerogels and the formation process of mullite. J Am Ceram Soc 69:652–656
Ortega A, Rouquerol F, Akhouayri S, Laureiro Y, Rouquerol J (1993) Kinetical study of the thermolysis of kaolinite between 30 and 1000 °C by controlled rate evolved gas analysis. Appl Clay Sci 8:207–214
Padlewsky S, Heine V, Price GD (1992) The energetics of interaction between oxygen vacancies in sillimanite: a model for the mullite structure. Phys Chem Minerals 19:196–202
Pask JA, Tomsia AP (1991) Formation of mullite from sol-gel mixtures and kaolinite. J Am Ceram Soc 74:2367–2373
Redfern SAT (1987) The kinetics of dehydroxylation of kaolinite. Clay Minerals 22:447–456
Rocha J, Klinowski J (1990) 29Si and 27Al magic-angle-spinning NMR studies of the thermal transformation of kaolinite. Phys Chem Minerals 17:179–186
Rodrigo PD, Boch P (1985) High purity mullite ceramics by reaction sintering. Int Journal High Technol Ceram 1:3–30
Suitch PR (1986) Mechanism for the dehydroxylation of kaolinite, dikite, and nacrite from room temperature to 455 °C. J Am Ceram Soc 69:61–65
Sundaresan S, Aksay IA (1991) Mullitization of diphasic aluminosilicate gels. J Am Ceram Soc 74:2388–2392
Toussaint F, Fripiat JJ, Gastuche MC (1963) Dehydroxylation of kaolinite. I. Kinetics. J Phys Chem 67:26–30
Wei WC, Halloran JW (1988) Transformation kinetics of diphasic aluminosilicate gels. J Am Ceram Soc 71:581–587
About this article
Cite this article
Gualtieri, A., Bellotto, M., Artioli, G. et al. Kinetic study of the kaolinite-mullite reaction sequence. Part II: Mullite formation. Phys Chem Minerals 22, 215–222 (1995). https://doi.org/10.1007/BF00202254
- Apparent Activation Energy
- Induction Time
- Defective Structure